Publisher’s version / Version de l'éditeur:
Acta Crystallographica Section B: Structural Science, B63, pp. 37-48, 2007
READ THESE TERMS AND CONDITIONS CAREFULLY BEFORE USING THIS WEBSITE. https://nrc-publications.canada.ca/eng/copyright
Vous avez des questions? Nous pouvons vous aider. Pour communiquer directement avec un auteur, consultez la
première page de la revue dans laquelle son article a été publié afin de trouver ses coordonnées. Si vous n’arrivez pas à les repérer, communiquez avec nous à PublicationsArchive-ArchivesPublications@nrc-cnrc.gc.ca.
Questions? Contact the NRC Publications Archive team at
PublicationsArchive-ArchivesPublications@nrc-cnrc.gc.ca. If you wish to email the authors directly, please see the first page of the publication for their contact information.
Archives des publications du CNRC
This publication could be one of several versions: author’s original, accepted manuscript or the publisher’s version. / La version de cette publication peut être l’une des suivantes : la version prépublication de l’auteur, la version acceptée du manuscrit ou la version de l’éditeur.
For the publisher’s version, please access the DOI link below./ Pour consulter la version de l’éditeur, utilisez le lien DOI ci-dessous.
Access and use of this website and the material on it are subject to the Terms and Conditions set forth at
Ab initio constrained crystal-chemical Rietveld refinement of
Mercier, Patrick H.J.; Dong, Zhili; Baikie, Thomas; Le Page, Yvon; White, T.
J.; Whitfield, Pamela S.; Mitchell, Lyndon
L’accès à ce site Web et l’utilisation de son contenu sont assujettis aux conditions présentées dans le site LISEZ CES CONDITIONS ATTENTIVEMENT AVANT D’UTILISER CE SITE WEB.
NRC Publications Record / Notice d'Archives des publications de CNRC:https://nrc-publications.canada.ca/eng/view/object/?id=477da056-12cf-42e7-964c-e0ecd2df1d20 https://publications-cnrc.canada.ca/fra/voir/objet/?id=477da056-12cf-42e7-964c-e0ecd2df1d20
Acta Crystallographica Section B
constrained crystal-chemical Rietveld
refinement of Ca10
Patrick H. J. Mercier,a* Zhili Dong,bThomas Baikie,bYvon Le Page,aT. J. White,bPamela S. Whitfieldaand Lyndon D. Mitchelc
Institute for Chemical Process and Environ-mental Technology (ICPET), National Research Council of Canada, Ottawa, Ontario, Canada K1A 0R6,bSchool of Materials Science and
Engineering, Nanyang Technological University, Singapore 639798, Singapore, andcInstitute for
Research in Construction (IRC), National Research Council of Canada, Ottawa, Ontario, Canada K1A 0R6
Correspondence e-mail: email@example.com
#2007 International Union of Crystallography Printed in Singapore – all rights reserved
Extraction of reliable bond distances and angles for Ca10(VxP1 xO4)6F2 apatites using standard Rietveld
refine-ment with Cu K X-ray powder data was significantly impaired by large imprecision for the O-atom coordinates. An initial attempt to apply crystal-chemical Rietveld refine-ments to the same compounds was partly successful, and exposed the problematic determination of two oxygen–metal– oxygen angles. Ab initio modeling with VASP in space groups
P63/m, P21/m and Pm showed that both these angular
parameters exhibited a linear dependence with the vanadium content. Stable crystal-chemical Rietveld refinements in agreement with quantum results were obtained by fixing these angles at the values from ab initio simulations. Residuals were comparable with the less precise standard refinements. The larger vanadium ion is accommodated primarily by uniform expansion and rotation of BO4tetrahedra combined
with a rotation of the Ca–Ca–Ca triangular units. It is proposed that the reduction of symmetry for the vanadium end-member is necessary to avoid considerable departures from formal valences at the AII and B sites in P63/m. The
complementarity of quantum methods and structural analysis by powder diffraction in cases with problematic least-squares extraction of the crystal chemistry is discussed.
Received 19 May 2006 Accepted 30 October 2006
Apatite-type structures combine crystallochemical flexibility with considerable durability, making them materials of interest for the long-term stabilization of toxic metals from municipal incinerators (Eighmy et al., 1998; Valsami-Jones et al., 1998; Crannell et al., 2000) and high-level nuclear waste (Ewing & Wang, 2002; Vance et al., 2003; Terra et al., 2006). The most common symmetry is P63/m, leading to the general formula
4][AII6][(BO4)6]X2, although numerous low-symmetry
derivatives have been reported. Topologically, apatites can be considered to be one-dimensionally microporous and zeolite-like, with a flexible framework created through the corner-connection of AIO6 metaprism columns with isolated BO4
tetrahedra. The channels are occupied by AII ions in the disposition of irregular AIIO6X polyhedra. A and B cation
ordering is observed on occasion and usually leads to a reduction of symmetry.
In solid solution fluorapatite [Ca10(PO4)6F2] can
accom-modate larger ions of valence 1+, 2+ and 3+ in place of Ca, and smaller 4+, 5+ and 6+ ions for P (White et al., 2005). While apatites have the potential to immobilize a spectrum of elements, compositional tailoring is nevertheless required, as their adaptability is constrained to suitable combinations of ions that maintain charge balance and accept the steric and topological limitations of the structure. A model involving
crystal chemical parameterization (Mercier, Le Page et al., 2005) was then implemented in scripts (Mercier et al., 2006a) for Rietveld refinement with powder diffraction data using
TOPAS(Bruker, 2005) with the goal of facilitating the design of eco-apatites as storage matrices. This approach has been complemented through the systematic exploration of apatite domains by the synthesis of a wide variety of substituted compounds (Dong et al., 2002; Dong & White, 2004a,b; Kim et
In this paper it is demonstrated that precise crystallographic information can be extracted from the X-ray diffraction profiles of vanadium-substituted fluorapatites (also known as fluorovanadinites) through constraining of the crystal-chemical refinement with the results of quantum mechanical optimization.
2.1. Sample synthesis and characterization
Eleven apatite powders of the Ca10(VxP1 xO4)6F2
solid-solution series (x = 0.0, 0.1, . . . , 1.0) were synthesized via solid-state chemical reaction. CaO (obtained by firing and decomposing AR-grade CaCO3 at 1173 K), V2O5 and CaF2
powders were mixed with dilute orthophosphoric acid in stoichiometric proportions and stirred at room temperature for more than 2 h. The sludge was dried at 368 K in an oven for 2 d, followed by heat treatment at 1173 K for 24 h. Detailed examination of the samples by scanning electron microscopy, energy-dispersive X-ray spectroscopy and mineralogical
observation with a polarizing microscope were consistent with complete reaction. We accordingly assumed compositions for the samples from the proportions of the reactants before synthesis.
2.2. Electron diffraction and imaging
An extensive search of all Ca10((VxP1 x)O4)6F2materials
was initiated by transmission electron microscopy (TEM) using a JEM-3010 instrument operated at 300 keV. For each sample, a small quantity of fluorovanadinite was lightly crushed under ethanol with an agate mortar and pestle, then dispersed ultra-sonically. Several drops of the suspension were depos-ited on holey-carbon coated copper grids and the crystal fragments oriented perpen-dicular to the tunnel direc-tion to search for V/P order. 2.3. X-ray powder diffrac-tion
Powder diffraction patterns were collected with a Shimadzu LabX XRD-6000 diffractometer (Bragg–Brentano geometry) equipped with a Cu K X-ray tube operated at 40 kV and 40 mA (Table 1). Samples were mounted in a top-loaded trough and were not rotated during data collection. Under these conditions the intensity of the strongest peak was 10 000–12 000 counts. Patterns for samples of the 11 compositions prepared in x2.1 were analyzed. Very minor impurity reflections of Ca3(PO4)2
and/or Ca3(VO4)2 were detected in the diffractograms for
samples of nominal compositions Ca10(PO4)6F2,
Ca10(V0.1P0.9O4)6F2 and Ca10(V0.9P0.1O4)6F2. All apatite
Instrument parameters used for X-ray powder diffraction Rietveld refinement.
Geometry: Bragg–Brentano Divergence slit: fixed = 1.0
Radiation source: Cu K Receiving slit: 0.3 mm Generator: 40 kV, 40 mA Detector: scintillation counter Tube: 12 mm long line focus Step size: 0.02
Scan mode: /2 Time per step: 10 s Secondary monochromator: graphite Angular range: 10–1402
Primary and secondary Soller slits: 6.0 Mean temperature of
measurement: 295 K
Summary of the parameters refined and derived for crystal-chemical (C-CH) and standard crystallographic (CRYS) refinement models.
Please refer to Table 1 in Mercier, Le Page et al. (2005) for all the parameter definitions and symbols, as well as all the equations necessary to obtain the parameters derived from those that are refined.
dAIO1, AIO, AI, AI, dB—O, O—B—O,
AII, AII, dAIIO3, ’O3AIIO3
a, c, AI
y, Bx, By,
O1x, O1y, O2x, O2y, O3x, O3y, O3z (Total = 10) (Total = 14)
a, c, AIO1, , AIz, AIIx, AIIy, Bx, By,
O1x, O1y, O2x, O2y, O3x, O3y, O3z
, AIO, A Iz¼0
AIO, AI, AI, hB—Oi,
hO—B—Oi, AII, (AII—X), AII, (AII—O3), ’O3AIIO3,
Illustration of the six possible atomic sites for the location of V atoms in
reflections could be assigned to P63/m symmetry, except for
the vanadium end-member where split peaks were indicative of lower symmetry.
2.4. Rietveld analysis
The software program TOPAS, Version 3.0 (Bruker, 2005), implementing the fundamental parameters approach (FPA; Cheary & Coelho, 1992) was used for Rietveld refinement. In the convolution-based profile-fitting process of the FPA (Kern
et al., 2004), the intensity profile is synthesized from the X-ray emission profile, the instrument parameters and specimen-dependent parameters. In addition to the integrated inten-sities and 2 positions of the diffraction lines, both diffract-ometer- and specimen-dependent parameters may be refined, and constitute the convolution parameters that are used to generate the aberration profiles. In the present work a common set of diffractometer-dependent variables (Table 1) were used with a full axial divergence model (Cheary & Coelho, 1998a,b). The specimen-dependent parameters which were refined were the zero error, a user-specified number of coefficients of a Chebyshev polynomial fitting the background, and the ‘Crystallite Size’ and/or ‘Microstrain’ parameters used to model microstructure-controlled line broadening.
Two types of Rietveld refinement modeling were used (Table 2):
(i) a standard crystal-lographic approach in
P63/m involving 14
crys-tallographic parameters (lattice parameters a and
c, 12 fractional atomic coordinates); (ii) a crystal-chemical determination where 10 parameters representing observed polyhedral distortions are directly refined by least-squares refinement (Mercier, Le Page et al., 2005; Mercier
et al., 2006a).
The F atoms were assumed to occupy a Wyckoff posi-tion of type 2(a) in P63/m
(x, y, z = 0, 0, 1/4; 0, 0, 3/4) for all refinements. In view of the compositional homogeneity observed in x2.1, occupancy factors were fixed at the nominal values of Ca10(VxP1 x
-O4)6F2, while refining only
the isotropic atomic displacement parameters (ADPs). A common isotropic ADP was assumed for the O1, O2 and O3 sites (beqO), whereas individual isotropic ADPs were refined for the AI, AIIand B cation sites (beqA1, beqA2, beqB; Table 2). On the basis of singular value decomposition (SVD) analyses of the least-squares normal-equations matrix performed using the program SVDdiagnostic (Mercier et al., 2006b), these two types of Rietveld refinement schemes were shown to have similar numerical stability for a high-quality X-ray powder data set of the fluorapatite end-member Ca10(PO4)6F2in Mercier et al. (2006a).
2.5. Ab initio modeling
The modeling and ab initio interface software environment
Materials Toolkit, Version 2.0 (Le Page & Rodgers, 2005; http://www.tothcanada.com/toolkit/), was used to prepare input files for ab initio total-energy minimization calculations. The crystallographic parameters arising from these calcula-tions for P63/m apatite end-member compositions
Ca10(PO4)6F2 and Ca10(VO4)6F2 were reported earlier
(Mercier, Le Page et al., 2005; Mercier, Whitfield et al., 2005) and are listed in Table 3 (supplementary material1
). To model
(a) A  through-focal series for disordered P63/m and ordered vanadium and phosphorus models of Ca10((V0.5P0.5)O4)6F2 calculated for a thickness of 47 A˚ using the multislice method as realised in JEMS (Stadelmann, 1987). Structures derived from X-ray determinations were used for the calculations. Microscope parameters were Cs= 1.4 mm, spread of focus = 10 nm, beam semi-convergence = 0.5 mrad. (b) A high-resolution image of a region in a crystal of nominal composition Ca10((V0.5P0.5)O4)6F2. Such images, which extended for many thousands of A˚ s, were characteristic of the crystals over the entire solid solution, indicating an absence of miscibility gaps that would promote the formation of phosphorous- or vanadium-rich nanodomains. (c) Comparison of the experimental and calculated images of the P21/m model of Ca10(VO4)6F2 (Dong & White, 2004b). The small departure from the hexagonal metric could not be distinguished in such images, but was apparent in selected-area diffraction patterns.
Supplementary data for this paper are available from the IUCr electronic archives (Reference: KD5006). Services for accessing these data are described at the back of the journal.
the solid-solution series, coordi-nate-only (CO) optimizations using experimental lattice parameters (Table 4 – see supplementary material) and cell-and-coordinate (CC) optimizations for materials with ideal compositions Ca10(V1/ 6P5/6O4)6F2, Ca10(V2/6
performed. Modeling for solid solutions began with a description in the space group P1 of the P63/m
structure of Ca10(PO4)6F2. In this
P1 model now containing six inde-pendent P atoms, we replaced the required proportion of P atoms by vanadium ones. This gave five ordered structures that we used as models for the corresponding solid solutions. Automated extraction of the symmetry of the V compounds by Materials Toolkit indicated the space group P21/m when there was
an even number of V atoms per cell [e.g. Ca10(VO4)2(PO4)4F2] and Pm
for the remainder (Fig. 1). For direct comparison of coordinates with previous work (Dong & White, 2004b), the b-unique P21/m
setting was transformed into the c-unique P1121/m setting, before
proceeding with ab initio optimi-zation. The lattice parameters used for CO optimizations were those determined experimentally for samples with nominal compositions closest to the ideal compositions used in the ab initio models for solid solutions; e.g. the experi-mental lattice parameters for the sample Ca10(V0.3P0.7O4)6F2 (Table
4 – see supplementary material) was used for CO optimization of the P1121/m model with the
(Table 3b – supplementary mate-rial).
VASP (Kresse, 1993; Kresse & Hafner, 1993, 1994) was used for all
ab initio calculations with the following common execution para-meters: GGA PAW potentials (Kresse & Joubert, 1999); elec-tronic convergence at 1 107eV; convergence for forces of 1 104eV A˚1;
Typical profile fits obtained for the different types of Rietveld refinement: (a) unrestrained and (b) restrained standard crystallographic refinement; (c) crystal-chemical refinement.
blocked iterative optimization of the wavefunctions in combination with reciprocal-space projectors (Davidson, 1983); reciprocal space integration with a Monkhorst–Pack
scheme (Monkhorst & Pack, 1976); a Methfessel–Paxton smearing scheme of the order 1 and width 0.2 eV for energy corrections (Methfessel & Paxton, 1989). Spin polarization corrections were not used. K-mesh dimensions of 2 2 3 and 2 3 2 were employed for
P1121/m and P1m1 models, respectively (Table
3 – supplementary material). A total of 20 to 35 single-point energy-minimization iterations were completed for each simulation to ensure proper convergence of atom relaxation, calcu-lated energy and stress. The calculations required approximately 2 d per structure on a single 3 gHz Athlon-64 PC running serial
VASP4.6.3 under Microsoft1 Windows1 XP, using the execution scheme described above. The resulting atomic coordinates and cell parameters are summarized in Table 3 (supplementary material), together with the total free-energy output for the final mini-mization cycles of each simulation.
3.1. Electron diffraction and imaging
Models computed through the focal series for the  zone axis of P63/m and P66 for
Ca10((V0.5P0.5)O4)6F2are shown as the top and
the bottom bands of Fig. 2(a), respectively. The high-resolution image shown in Fig. 2(b) is a typical example of a structure projection along  for the preparation with the nominal composition Ca10((V0.5P0.5)O4)6F2. In Fig. 2(c)
a  high-resolution picture for Ca10(VO4)6F2 is compared with simulated
images using the P21/m model proposed earlier
by Dong & White (2004b).
3.2. Extraction of crystal chemistry by stan-dard Rietveld refinement
Unrestrained and restrained standard Riet-veld refinements were performed for all compositions except the vanadium end-member (Table 4 – supplementary material). Typical profile fits are shown in Fig. 3. The restraints were implemented by applying the ‘Parabola_N’ penalty function of TOPAS so that the B-site cations were soft-constrained to a distance ro= 1.54 + (1.74 1.54)x A˚ away
from their four nearest-neighbor O atoms, the values being selected on the basis of the stan-dard ionic radii (Shannon, 1976). Table 5 (supplementary material) summarizes the crystal-chemical parameters extracted from standard Rietveld refinement results (Table 4 – supplementary material) using the equations given in Table 1(b) of Mercier, Le Page et al.
Crystal-chemical parameters extracted from unrestrained (open symbols) and restrained (filled symbols) standard Rietveld refinement results (Table 4 – see supplementary material) using the equations given in Table 1(b) of Mercier, Le Page et al. (2005).
(2005). Fig. 4 plots these indirectly determined crystal-chemical parameters obtained by the analysis of fractional atomic coordinates and lattice parameters (Table 4 – see supplementary material) as a function of the vanadium frac-tion x. It is apparent that, as far as the extracfrac-tion of the crystal chemistry is concerned, unrestrained versus restrained stan-dard refinements show approximately the same overall variation of parameter values and systematic trends across the solid-solution series.
3.3. Direct least-squares refinement of crystal-chemical parameters
An initial attempt at simultaneous direct least-squares determination of all 10 crystal-chemical parameters yielded structures with reasonable bond distances and angles. However, SVD analysis of the least-squares normal equation matrix indicated that the O—B—Oand ’O3AIIO3 bond-angle
parameters (Table 2) were the main components of eigen-vectors associated with small singular values, meaning that their standard uncertainty (s.u.) would be large and therefore that their numerical values would be extracted with poor precision. We accordingly performed tests where we imposed values for O—B—Oor ’O3AIIO3. We observed that quite a
large range of values could be imposed in this way with no meaningful change in residuals, goodness-of-fit or other agreement factors, but with clear repercussions for values extracted for the eight remaining parameters. This kind of behavior is presumably caused by the fact that the singular vectors are mostly but not entirely along the variables O—B—O
or ’O3AIIO3. Imposed changes in the numerical values of
those variables can then be compensated for by changes in other refinement variables, without a significant change in the agreement factors. Whatever its cause, this kind of behavior of the least-squares refinement is most worrying for the extrac-tion of meaningful crystal-chemical parameters.
3.4. Ab initio optimized values for sO—B—Oand uO3AIIO3
In order to better condition the crystal-chemical refine-ment, numerical values derived from ab initio total-energy minimization calculations (Table 3 – supplementary material) were imposed on the bond-angle parameters O—B—O and
’O3AIIO3. Selected bond distances and angles (Table 6 –
supplementary material) for individual crystallographic sites of P1m1 and P1121/m ab initio optimized structures show that
the mean O—B—O and O3—AII—O3 oxygen–cation–oxygen
bond angles display a linear behavior when plotted against the vanadium fraction x (Fig. 5).
3.5. Ab initio constrained crystal-chemical refinement Imposing O—B—O and ’O3AIIO3 values from ab initio
simulations produced stable crystal-chemical Rietveld analyses, i.e. normal least-squares matrices with condition numbers sufficiently high to ensure precise and stable evaluation of refinement variables (Mercier et al., 2006b). Fig. 6 plots the eight crystal-chemical parameters (Table 7 – supplementary material) obtained by direct least-squares extraction for the solid-solution series by imposing values read off the linear relationships of Fig. 5 to bond-angle parameters ’O3AIIO3and O—B—O. Note that Figs. 4 and 6 are shown on
the same overall scales for the corresponding parameters.
Mean values of (a) O3—AII—O3 and (b) O—B—O oxygen–cation– oxygen bond angles for given ab initio structures as a function of the vanadium fraction x.
4.1. Electron diffraction and imaging
The large difference in ionic radii (Shannon, 1976) of tetrahedrally coordinated P5+ (0.17 A˚ ) and V5+ (0.355 A˚ ) raises the possibility of ordering, which in the simplest case of Ca10(PO4)3(VO4)3F2would result in alternate phosphorus and
vanadium in successive atomic planes perpendicular to the channels, an ordering which results in the space group P66. In principle, this symmetry is readily distinguished from P63/m in
the  or  zone axes as 00l, l = 2n, reflections will be absent only when the screw axis is present. However, in selected-area electron diffraction, the superposition of double diffraction reflections makes such analyses problematic, and convergent-beam electron diffraction that would limit this effect may be compromised by the reduction of V5+ and crystallographic alteration to perovskite under a focused elec-tron beam (Dong et al., 2005). Direct imaging of the tetrahedral sites also proves incon-clusive, as simulations show the averaged projected potential of overlaid phosphorus and vanadium is indistinguishable in either the P63/
mor P66 models (Fig. 2a). There remains the prospect that compositionally elicited nano-domains 50–1000 A˚ in extent may exist, as observed in natural apatite (Ferraris et al., 2005) and plumbous vanadinites (Dong & White, 2004a). Domains were not detected in any samples, with the projected structures appearing to be very homogeneous – a typical example for the preparation of nominal composition Ca10((V0.5P0.5)O4)6F2 is shown in
Fig. 2(b). Similarly, the reduction of symmetry to P21/m that was proposed earlier (Dong &
White, 2004b) for Ca10(VO4)6F2 was not
distinguishable by high-resolution imaging (Fig. 2c).
4.2. Crystal-chemical versus standard Rietveld refinement results
In comparing the systematics arising from crystallographic (Table 4 – supplementary material – Fig. 3) versus crystal-chemical (Table 7 – supplementary material, Fig. 6) Rietveld refinement, the most striking obser-vations are as follows: First, inverse solid-solution systematics (Fig. 4c versus Fig. 6b) were extracted for the counter-rotation angle AI (Table 2, Fig. 7). The latter parameter is
equivalent to the AIO
6metaprism twist angle ’
(’ = 602
AI) first defined by White & Dong
(2003). As a classification of the apatites based on the metaprism twist ’ has been presented in White et al. (2005), it becomes important to ascertain which of the two sets of values extracted for AI are reliable. Fig. 7 compares
the set values with the correlation AI versus
’O3AIIO3observed by Mercier, Le Page et al.
(2005) for accurate single-crystal refinements and ab initio simulations of the known P63/m
end-member structures. It is shown that AI
values extracted by crystal-chemical
Crystal-chemical parameters (Table 7 – see supplementary material) obtained by direct least-squares extraction for the solid-solution series by imposing the linear relationships of Fig. 3 to bond-angle parameters ’O3AIIO3and OBO.
ment are in better general agreement with the trend in Mercier, Le Page et al. (2005) than those obtained from standard crystallographic refinement results. As the trend was established with intrinsically more accurate single-crystal data, it is concluded that the crystal-chemical refinement method provides a more accurate quantitative crystal-chemical analysis of the AIO6 metaprism twist angle than a standard
refinement of the same data.
It is also observed that variations of interatomic distance parameters for calcium–oxygen bonds in the AIand AIIsites are much larger in the standard refinements (Figs. 4a, b and i) than in their crystal-chemical counterparts (Figs. 6a, c and 6f). In comparing results from crystal-chemical versus standard crystallographic types of refinement using a high-quality fluorapatite X-ray powder data set, Mercier et al. (2006a) observed similar magnitudes of interatomic distance varia-tions by performing numerous refinements of the same experimental data with the addition of artificial random intensity noise, indicating a precision which is nearly an order of magnitude greater for crystal-chemical refinement than for standard crystallographic Rietveld analysis. This means that the range of values extracted here for interatomic distance parameters involving calcium–oxygen bonds in the AIand AII sites, by both unrestrained and restrained standard Rietveld refinement, varies somewhat from data set to data set. On the other hand, crystal-chemical refinement results indicate only a small data-set-to-data-set variation across the solid solution for the bond-length difference AIO between AI—O1 and AI—O2 bonds, and almost no significant variation for the AI—
O1 and AII—O3 bond lengths. As discussed below in x4.5, the
apparent difficulty in quantitative evaluation of interatomic distances for calcium–oxygen bonds in AIand AIIsites can be attributed to the poor precision in resolving oxygen positions
Comparison of AI values extracted by crystal-chemical versus standard crystallographic Rietveld refinements for the solid solution with the correlation AI versus ’O3AIIO3 observed by Mercier et al. (2005) for accurate single-crystal refinements and ab initio simulations of the known
P63/m end-member structures.
Diagrams showing the main geometric rearrangements that take place as more and more vanadium is substituted in the fluorapatite structure.
with conventional X-ray Rietveld refinement in the presence of heavy elements. The same remark applies to the lower accuracy in the determination of the AIO6 metaprism twist
angle ’ by standard crystallographic refinement.
4.3. Crystal-chemical systematics of vanadium-substituted fluorapatites
The present analysis allows the systematic tracking of structural modifications in fluorapatite when phosphorus is progressively replaced by larger vanadium (Fig. 8). As the vanadium content increases, the concomitant geometric re-arrangements include:
(i) a rotation (Fig. 8) and a uniform expansion of BO4
tetrahedra that take place through a linear increase of the B— O bond lengths (Figs. 4e and 6e), accompanied by minor ( 1) bending of O—B—O bond angles (Figs. 4f and 5b);
(ii) bond-stretching adjustment of the CaIO6 polyhedra
(Figs. 4a and b, and 6a and c), which elongate through varia-tion in the AIO1 angle (Table 7 – supplementary material;
Fig. 8), slightly twist through the counter-rotation angle AII
(Fig. 7) and rotate by an angle AI;
(iii) an expansion of the edges of the Ca—Ca—Ca triangles AII (Figs. 4g and 6g) and rotation away from the BO4
tetra-hedra through AII (Fig. 8). The angle AII progressively
increases towards a value of 120for large vanadium contents
(Figs. 4h and 6h).
By plotting the angle AII as a function of the ’O3AIIO3
bond angle (Fig. 9) for ab initio simulation results and published single-crystal work of a wide selection of P63/m
apatite end-members, it was found that there is a gap at around AII = 120 in an otherwise dense plot (Mercier, Le
Page et al., 2005). In terms of the present experiments, it is significant that the observed AII values for the phosphorus–
vanadium solid solution (Figs. 4g and 6h) move inside this gap as the vanadium content increases. In addition, the refine-ments show that:
(i) the refined microstrain parameters (Tables 2 and 4 from the supplementary material) for Ca10(VxP1 xO4)6F2samples
with x = 0.0–0.9 correlate directly with the vanadium fraction
(ii) the X-ray powder pattern for the Ca10(VO4)6F2
end-member is clearly of lower-symmetry, in line with previous work (Kreidler & Hummel, 1970; Dong & White, 2004b). It is proposed, therefore, that as the AII angle approaches
120for large vanadium content, a lowering of the symmetry is
induced. The steady trend in refined strain parameters versus vanadium content, as opposed to a maximum around x = 0.5 composition that is expected for solid solutions, is presumably an additional indication of the nearby symmetry transforma-tion.
4.4. Promoting symmetry reduction of metal-substituted fluorapatites
An empirical analysis of the driver for a phase transfor-mation to lower symmetry can be gained by considering the bond-valence sums (BVS) at the sites AI, AIIand B (Fig. 10, Table 8 – supplementary material). For the pure phosphate, Ca2+fits neatly in the AIIsite with a BVS of +2 v.u. (valence units), while it is somewhat compressed at site AI (BVS > +2 v.u.). As the vanadium content increases, the bond length of the BO4tetrahedron increases as expected (Figs. 4e and 6e),
Bond-valence sums (BVS) at sites AI , AII
and B (Table 8 – supplementary material) plotted as a function of the vanadium fraction x.
and causes a parallel increase in the average metal–anion bond length (hM—Ai) of the AI and AII sites (Table 8 – supplementary material). At the highest vanadium contents, just prior to the phase change in the Ca10(VO4)6F2
end-member, Ca2+ matches the AIsite interstice, while it is now somewhat small for the expanded AII site (BVS < +2 v.u.). Similarly, the tetrahedral B site is slightly stretched at the P end-member (BVS < 5 v.u.) and quite compressed (BVS > 5 v.u.) just before the symmetry change at the V end-member. While these departures from ideal valences are not unex-pected, the deviations of the BVS observed at the AIIand B
sites become exceptionally large at high vanadium content. This suggests that the phase transformation is promoted by the need to relax O atoms toward AIIsites and away from B sites.
A bond-valence analysis of the monoclinic P1121/m model for
Ca10(VO4)6F2 in Dong & White (2004b) indeed indicates
significant relaxation at the V site, and to a lesser degree at the
AII site, although further work is needed to establish the generality of this interpretation.
As valence summation indicates extension stress on the AII site in the vanadate-rich region, it follows that divalent ions of radius slightly larger than Ca2+, such as Pb2+, would prefer-entially occupy the AIIsite and stabilize the hexagonal phase by reducing the stress on site AII. This rationalization appears to be qualitatively supported by experiment as Pb2+ in
(PbxCa10 x)(VO4)6F2 (Dong & White, 2004a,b) is seen to
both preferentially occupy AII and stabilize the hexagonal
4.5. Complementarity of quantum methods and structure analysis by X-ray powder diffraction
Although the observations made here apply specifically to the Rietveld extraction of the crystal chemistry of vanadium-substituted fluorapatites, the approach is generally applicable to Rietveld refinements of moderately complex metal-oxide systems. SVD analysis of the normal matrix of Rietveld least-squares (Mercier et al., 2006b) indicates that singular values associated with some variables or singular combinations of variables are small, both for standard crystallographic refine-ment and for crystal-chemical refinerefine-ment (Mercier et al., 2006a). These singular values are the inverse of the variance of the corresponding variable or combination of variables, which means that some aspects of geometry and therefore crystal chemistry will be determined imprecisely. With standard crystallographic refinement of metal oxides with sealed-tube X-ray data, the O-atom coordinates are presumably in a category of variables associated with eigenvectors having weak eigenvalues compared with those of eigenvectors corresponding to unit-cell parameters and heavy-element coordinates. As the crystal chemistry of metal oxides is rationalized in terms of distortions and rotations of oxide polyhedra, it follows that the crystal chemistry extracted by crystallographic Rietveld refinement of conventional X-ray data will inevitably be compromised by the inherent difficulty in refining the oxygen coordinates demonstrated by SVD
analysis of refinement matrices. While crystal-chemical refinements also include combinations of variables with small singular values, there are fewer of them compared with stan-dard crystallographic refinements, but the extracted crystal chemistry is only marginally superior. Extraction of useful crystal chemistry by Rietveld profile analysis of sealed-tube X-ray data from metal oxides should therefore be performed with caution.
Reliability can be enhanced by considering that in crystal-chemical refinements all crystal-crystal-chemical variables are alge-braically independent in the model, but do not have the same degree of interpretability. Metal–oxygen distances are often interpreted in terms of bond valence (Brown & Altermatt, 1985) or by comparison with tables of ionic radii (Shannon, 1976). In the same way, polyhedral rotations may be intuitively understood in terms of steric effects within the structure. However, crystal-chemical instinct is often insufficient for rational interpretation of oxygen–cation–oxygen bond angles. In the case of apatite, the introduction of such crystal-chemical parameters in the model was essential to establish algebraic equivalence with the crystallographic description of the structure. Fortunately, bond angles and polyhedral rotations are accurately reproduced by ab initio optimization of the corresponding structure models, as demonstrated through comparisons with published accurate single-crystal work (Mercier, Le Page et al., 2005). A rational approach then is to fix one or more of those oxygen–metal–oxygen angles at values calculated through ab initio modeling, in order to better condition the Rietveld refinement. Hopefully, this would in turn allow the extraction of useful experimental values for the
remaining crystal-chemical variablesfrom conventional X-ray powder diffraction data.
The present study is a successful application of this proce-dure to combine the strengths of a variety of methods in different steps in the derivation. Instead of extracting metal– oxygen distances and angles from the poorly determined variables of standard crystallographic refinements, crystal-chemical refinement considers interatomic distances and angles to be variables in their own right, thus decreasing the possibility of incorrect derivation. It is well known that density-functional theory (DFT) quantum modeling may not be adequate to accurately determine bond lengths because the numerical accuracy of ab initio ‘potentials’ used to describe the electronic core is not yet quite sufficient for this purpose. However, DFT has proved reliable at modeling small struc-tural adjustments, as shown by the success of the quantum extraction of elastic tensor coefficients (see e.g. Le Page & Rodgers, 2005, and references therein), as this method establishes with considerable accuracy the minimum-energy configuration of valence electrons through hybridization of electronic orbitals. It is this hybridization that controls the bond-bending or polyhedral-rotation angles of the type that cannot be precisely obtained by Rietveld refinement of data from a sealed X-ray tube. In summary, this asset of DFT modeling can be used to compensate for the corresponding limitation of X-ray refinement, leading to better-conditioned crystal structure determinations, providing a route for the
derivation of more precise experimental values for the refinement variables that the crystal chemist needs most.
It can be argued that the more precise values derived in this way are somewhat less experimental than other values derived by full refinement of all possible variables in a standard crystallographic refinement, including atom occupancies, anisotropic atom displacements, extinction etc. The results of such unbiased refinements on our measured Cu K powder data sets would also have been inappropriate for the purpose of correctly extracting the crystal chemistry. This is because the imprecision of O-atom coordinates would have been made worse by the introduction of additional refinement para-meters, leading to inconclusive results. Treatment of standard refinement analogous to the procedure we have followed for crystal-chemical refinement would probably have resulted in our accepting metal positions from the X-ray Rietveld refinement while imposing O-atom positions from DFT opti-mization. For the extreme case where all oxygen coordinates would have been imposed in this way to obtain a stable and precise evaluation of remaining refinement variables, the extracted crystal chemistry could then hardly be called experimental because it would mostly be from DFT calcula-tions. In this regard, the ab initio constrained crystal-chemical refinement approach developed here is then a way to extract as much experimental crystal chemistry as possible, but the Cu K X-ray powder profile we could produce was still borderline. Under the circumstances, it seemed justified to have made the few simplifying and plausible assumptions detailed above, the reason being that these assumptions ended up making the difference between an unbiased but also inconclusive study and the plausibly constrained conclusive experimental crystal-chemical results reported here.
The remaining freely refined crystal-chemical parameters extracted from experimental profile measurements in no way contradict the DFT model optimized from theory. In other words, we almost reached the goal of most experiments: to perform a measurement, interpret it with a model in the light of existing theory down to the precision of the measurement and to derive useful conclusions from this interpretation. If we accept that the precision of the measurements is indicated by the agreement factors obtained with standard refinement of the same data, we have essentially achieved that goal of exhausting the precision in the data with a model that agrees with theory. Experimental results and those of DFT compu-tations buttress each other here and reinforce our trust both in the conclusions of the experimental study and in the sound-ness of the principles and approximations at the root of DFT software. It has helped significantly to be able to stabilize a least-squares system with partial results from DFT theory, and then observe agreement between theory and experiment over the remaining refinement parameters within the limitations of each approach. Known current deficiencies of DFT are not built into the method and there is progress each year in this area. It is currently too early to attempt to derive from theory alone structural information that can also be extracted experimentally. We nevertheless trust that, similar to what is already happening with the elasticity of materials (see e.g. Le
Page & Rodgers, 2005, and references therein), the day will come for the design work of materials because computations are already much cheaper than experiment for moderately large systems. The present study is hopefully a step in that direction.
By imposing results of quantum modeling in a crystal-chemical Rietveld refinement, a precise description of the vanadium-substituted fluorapatites has been obtained. Replacement of P5+by V5+is accommodated primarily by uniform expansion
and rotation of BO4tetrahedra combined with a rotation of
the Ca—Ca—Ca triangular units through the angle AII
defined in Mercier, Le Page et al. (2005). It is postulated that the reduction of symmetry for vanadium-rich apatite arises because:
(i) the angle AIIfor the solid solution approaches a value of
(ii) significant departures from formal valence at the AIIand
The novel approach of combining crystal-chemical Rietveld refinement and quantum calculations developed and imple-mented here is in general well suited for the precise investi-gation of the crystal chemistry of metal oxide compounds and their solid solutions.
This work was supported through the NRC/A*STAR Joint Research Programme on ‘Advanced Ceramic Methods for the Co-stabilization and Recycling of Incinerator Fly Ash with Industrial Wastes’. We thank Wang Lee Chin from the X-ray Diffraction Facility at NTU for collecting the diffraction patterns.
Brown, I. D. & Altermatt, D. (1985). Acta Cryst. B41, 244–247. Bruker (2005). TOPAS, Version 3.0. Bruker AXS, Karlsruhe,
Cheary, R. W. & Coelho, A. (1992). J. Appl. Cryst. 25, 109–121. Cheary, R. W. & Coelho, A. (1998a). J. Appl. Cryst. 31, 851–861. Cheary, R. W. & Coelho, A. (1998b). J. Appl. Cryst. 31, 862–868. Crannell, B. S., Eighmy, T. T., Krzanowski, J. E., Eusden Jr, J. D.,
Shaw, E. L. & Francis, C. A. (2000). Waste Manage. 20, 135–148. Davidson, E. R. (1983). Methods in Computational Molecular
Physics, edited by G. H. F. Diercksen & S. Wilson, Vol. 113, NATO Advanced Study Institute, Series C, p. 95. New York: Plenum Press.
Dong, Z. & White, T. J. (2004a). Acta Cryst. B60, 138–145. Dong, Z. & White, T. J. (2004b). Acta Cryst. B60, 146–154.
Dong, Z., White, T. J., Sun, K., Wang, L. M. & Ewing, R. C. (2005). J.
Am. Ceram. Soc. 88, 184–190.
Dong, Z., White, T. J., Wei, B. & Laursen, K. (2002). J. Am. Ceram.
Soc. 85, 2515–2522.
Eighmy, T. T., Crannell, B. S., Krzanowski, J. E., Butler, L. G., Cartledge, F. K., Emery, E. F., Eusden Jr, J. D., Shaw, E. L. & Francis, C. A. (1998). Waste Manage. 18, 513–524.
Ewing, R. C. & Wang, L. (2002). Reviews in Mineralogy and
Geochemistry, Vol. 48, Phosphates: Geochemical, Geobiological,
Hughes, pp. 673–700. Mineralogical Society of America and Geochemical Society, Washington, DC.
Ferraris, C., White, T. J., Ple´vert, J. & Wegner, R. (2005). Phys. Chem.
Miner. 32, 485–492.
Kern, A., Coelho, A. A. & Cheary, R. W. (2004). Diffraction Analysis
of the Microstructure of Materials, edited by E. Mittemeijer & P. Scardi, pp. 17–50. Berlin: Springer-Verlag.
Kim, J. Y., Dong, Z. & White, T. J. (2005). J. Am. Ceram. Soc. 88, 1253–1260.
Kreidler, E. R. & Hummel, F. A. (1970). Am. Mineral. 55, 170–184. Kresse, G. (1993). PhD thesis. Technische Universita Wien, Austria. Kresse, G. & Hafner, J. (1993). Phys. Rev. B, 48, 13115–13118. Kresse, G. & Hafner, J. (1994). Phys. Rev. B, 49, 14251–14269. Kresse, G. & Joubert, J. (1999). Phys. Rev. B, 59, 1758–1775. Le Page, Y. & Rodgers, J. (2005). J. Appl. Cryst. 38, 697–705. Mercier, P. H. J., Le Page, Y., Whitfield, P. S. & Mitchell, L. D (2006a).
J. Appl. Cryst. 39, 369–375.
Mercier, P. H. J., Le Page, Y., Whitfield, P. S. & Mitchell, L. D (2006b).
J. Appl. Cryst. 39, 458–465.
Mercier, P. H. J., Le Page, Y., Whitfield, P. S., Mitchell, L. D., Davidson, I. J. & White, T. J. (2005). Acta Cryst. B61, 635– 655.
Mercier, P. H. J., Whitfield, P. S., Mitchell, L. D., Davidson, I. J., Le Page, Y. & White, T. J. (2005). Advances in Ecomaterials – 7th
International Conference on Ecomaterials (ICEM7) and 3rd International Conference on Materials for Advanced Technologies (ICMAT 5005), edited by T. White et al., Vol. 2, pp. 396–401. Singapore: Stallion Press (S) Pte Ltd.
Methfessel, M. & Paxton, A. T. (1989). Phys. Rev. B, 40, 3616–3621. Monkhorst, H. J. & Pack, J. D. (1976). Phys. Rev. B, 13, 5188–5192. Shannon, R. D. (1976). Acta Cryst. A32, 751–767.
Stadelmann, P. A. (1987). Ultramicroscopy, 21, 131–146.
Terra, O., Dacheux, N., Audubert, F. & Podor, R. (2006). J. Nucl.
Mater. 352, 224–232.
Valsami-Jones, E., Ragnarsdottir, K. V., Putnis, A., Bosbach, D., Kemp, A. J. & Gressey G. (1998). Chem. Geol. 151, 215–233. Vance, E. R., Ball, C. J., Begg, B. D., Carter, M. L., Day, R. A. &
Thorogood, G. J. (2003). J. Am. Ceram. Soc. 86, 1223–1225. White, T. J. & Dong, Z. (2003). Acta Cryst. B59, 1–16.
White, T. J., Ferraris, C., Kim, J. & Madhavi, S. (2005). Apatite – An
Adaptive Framework Structure, in Reviews in Mineralogy and Geochemistry, Vol. 57, Micro- and Mesoporous Mineral Phases, edited by G. Ferraris & S. Merlino, pp. 307–373. Mineralogical Society of America and Geochemical Society, Washington, DC.